Strength of Bolted Timber Connections with Steel Side Members · PDF file bolted connections...
Embed Size (px)
Transcript of Strength of Bolted Timber Connections with Steel Side Members · PDF file bolted connections...
United States Department of Agriculture
Forest Products Laboratory
Strength of Bolted Timber Connections with Steel Side
Paper FPL-RP-513 Members
T. L. Wilkinson
This study investigated the properties of bolted tim- ber connections with steel side members. The intent of this study was to determine (1) how well the Euro- pean Yield Model (EYM) predicts experimental results (2) if there is a difference in results from tension- and compression-loaded specimens, and (3) what the effect is of steel side member thickness. Three bolt diame- ters and four ratios of main member thickness to bolt diameter were investigated. Connections were loaded both parallel and perpendicular to the gram. Results were compared to predicted results from the EYM. The study revealed that the EYM predicts connection yield load with acceptable accuracy.
Keywords: Bolts, wood connections, European Yield Model, yield load, dowel embedment strength
Wilkinson, T. L. 1992. Strength of bolted timber con- nections with steel side members. Res. Pap. FPL-RP- 513. Madison, WI: U.S. Department of Agriculture, Forest Service, Forest Products Laboratory. 10 p.
A limited number of free copies of this publication are available to the public from the Forest Products Labo- ratory, One Gifford Pinchot Drive, Madison, WI 53705- 2398. Laboratory publications are sent to more than 1,000 libraries in the United States and elsewhere.
The Forest Products Laboratory is maintained in coopera- tion with the University of Wisconsin.
Strength of Bolted Timber Connections With Steel Side Members
T. L. Wilkinson, Research General Engineer Forest Products Laboratory, Madison, Wisconsin
Historically, design values for bolted timber connec- tions (NFPA 1986) have been based on research con- ducted by Trayer (1932). Trayer’s recommendations were based on an empirical fit of experimental data and thus are limited to the connection geometries evaluated, although Trayer’s recommendations have been extrapo- lated to other geometries by rule of thumb type proce- dures. Trayer empirically related bolt bearing stress at proportional limit with the ratio of main member thick- ness to bolt diameter. He further related the bolt bear- ing stress with the small, clear compressive strength of the wood. His sample sizes were four and five specimens.
Doyle and Scholten (1963) evaluated bolted connections in Douglas-fir with sample sizes of three specimens. Soltis and others (1986) evaluated bolted Douglas-fir connections with wood side members using sample sizes of 16 specimens. Both of these studies found that the previous recommendations from Trayer were still valid.
In recent code developments, the European Yield Model (EYM) proposed by Johanson (1949) has been adopted as the base for predicting the strength of bolted connections. The EYM can predict the strength for various connection geometries and material com- binations for two- and three-member connections. Soltis and others (1986) found that the EYM explains much of the observed behavior of bolted timber con- nections. McLain and Thangjitham (1983) also found that the EYM predicts bolted connection performance. These studies indicated that the EYM can be a useful model to predict connection behavior for single-bolted connections.
Most investigations of bolted timber connections have used small sample sizes that do not allow the calcula- tion of reliable statistical properties of the distribution of connection properties. In the future, design loads for bolted connections may be derived using reliability-
based design procedures, which would require distribu- tion properties.
Most studies have reported only proportional limit loads for bolted timber connections. For future design procedures, other connection properties may need to be known. These properties include maximum load and connection deformation information. Deformation data would be useful in setting serviceability limits for con- nections in a reliability-based design procedure. De- formation data are also needed for predicting the load distribution among bolts in multiple bolt connections in procedures such as that developed by Lantos (1969).
This paper presents data for single-bolted timber con- nections with steel side members. Input data for use with the EYM are also presented and EYM-predicted loads are compared to experimental results. The objec- tives were to determine (1) how well the EYM predicts experimental results, (2) if results from tension-loaded specimens differ from results from compression-loaded specimens, and (3) what the effect is of steel side mem- ber thickness.
European Yield Model
The EYM provides an analysis method to predict the strength of a two- or three-member dowel-type connec- tion. It was originally developed in Europe (Johanson 1949) and is based on equilibrium equations resulting from the free body diagram of a bolt in a wood mem- ber. The method has been examined by McLain (1983) and Soltis (1986). Both found general agreement be- tween predicted and experimental data sets.
The EYM assumes that the capacity of a bolted con- nection is attained when either (1) the compressive strength of the wood beneath the bolt is exceeded (Mode I or II yielding) or (2) one or more plastic hinges develop in the bolt (Modes III or IV yielding).
These assumptions provide for several modes of yielding diameter. Steel side member thickness was 1/4 in. depending on connection member dimensions, member (6.4 mm), 3/8 in. (9.5 mm), and 1/2 in. (12.7 mm) strength, and bolt strength. For three-member connec- for the 1/2-in. (12.7-mm) bolts; 3/8 in. (9.5 mm) for tions, the yield load Zy is the smallest value given by the 3/4-in. (19.0-mm) bolts; and 1/2 in. (12.7 mm) for the following equations. the 1-in. (25.4-mm) bolts.
Mode I,,, (1a) The wood main members were cut from Douglas-fir glulam beams constructed of L2 or better grade lami- nating stock. Specimens with 1/2-in. (12.7-mm) bolts had two laminations, those with 3/4-in. (19.0-mm) bolts had three laminations, and those with 1-in. (25.4- mm) bolts had four laminations. All laminations were 1-1/2 in. (38.1 mm) thick. Bolt holes 1/16 in. (1.6 mm) greater than the bolt diameter were drilled parallel to the glue lines. All wood members had a moisture content of approximately 12 percent.
Mode I, ( lb)
Mode IV (1d)
Re is Fem /Fes,
Rt tm/ts ,
tm thickness of main member (in.),
t s thickness of side member (in.),
Fe m dowel bearing strength of main member (lb/in2),
Fes dowel bearing strength of side member (lb/in 2),
Fy bending yield strength of bolt (lb/in 2), and
D bolt diameter (in.).
(Conversion factors are 1 in. = 25.4 mm; 1 lb/in2 = 6.89 kPa.)
M e t h o d s
Three-member connections loaded both parallel and perpendicular to the grain were evaluated. Each con- nection consisted of a wood main member and steel side members fastened with a single bolt.
Three bolt diameters, 1/2 in. (12.7 mm), 3/4 in. (19.0 mm), and 1 in. (25.4 mm), were used. The steel bolts were SAE Grade 2. Bolts were long enough to prevent bearing on the threads. Nuts were finger tight at time of test.
Ratios of main member thickness to bolt diameter (tm /D) were 3.0, 5.125, 6.75, and 10.25 for each bolt
Twenty replications were created for each combination of variables for a total of 240 parallel-to-grain loaded specimens and 240 perpendicular-to-grain loaded specimens.
The connection configurations were made to exceed National Design Specification (NFPA 1986) require- ments for end and edge distance. The distance from the bolt to the end of the main member was 7.5 times the bolt diameter for parallel-to-grain loading. The dis- tance from the bolt to the loaded edge exceeded 4.25 times the bolt diameter for perpendicular-to-grain load- ing. Edge distance equaled or exceeded 1.5 times the bolt diameter for both loadings. For perpendicular-to- grain loading, the distance between supports was 9 in. (230 mm) for specimens with 1/2-in. (12.7-mm) bolts, 13.5 in. (340 mm) for specimens with 3/4-in. (19.0. mm) bolts, and 18 in. (460 mm) for specimens with 1-in. (25.4-mm) bolts. These distances were 3 times the depth of the main member, as specified by ASTM D1761-88 (ASTM 1990).
In addition to the main series of teats, 20 parallel-to- grain loaded specimens were evaluated using compres- sion loading instead of tension loading. These speci- mens used 3/4-in. (19.0-mm) bolts and a tm/D of 6.75. Two additional groups of 20 parallel-to-grain loaded specimens each were evaluated with 1/2-in. (12.7- mm) bolts and steel side member thicknesses of 3/8 in. (9.5 mm) and 1/2 in. (12.7 mm). For these two groups the tm /D was 5.125.
The test procedures for parallel-to-grain loading (Fig. 1) and perpendicular-to-grain loading (Fig. 2) generally followed those given in ASTM D1761-88 (ASTM 1990). Tension loading was used with the parallel-to-grain loaded specimens except for one group, which used compression loading. The applied load was
Figure 2—Experimental arrangement for loading bolted connections perpendicular to grain.
Figure 1—Experimental arrangement for loading bolted connections parallel to grain.
deformation controlled at either 0.035 or 0.050 in/min (0.89 or 1.27 mm/min). The tests were terminated when failure occurred.
Deformation was measured using linear variable dif- ferential transd